# Dislocation Density Crystal Plasticity Based Finite Element Modeling

date post

31-Dec-2016Category

## Documents

view

221download

6

Embed Size (px)

### Transcript of Dislocation Density Crystal Plasticity Based Finite Element Modeling

DISLOCATION DENSITY CRYSTAL PLASTICITY BASED FINITE ELEMENT

MODELING OF ULTRASONIC CONSOLIDATION

D. Pal*, B. E. Stucker+

*Department of Mechanical & Aerospace Engineering, Utah State University, Logan, UT 84322 +Department of Industrial Engineering, University of Louisville, Louisville, KY 40292

Abstract

A dislocation density based constitutive model has been developed and implemented into

a crystal plasticity quasi-static finite element framework. This approach captures the statistical

evolution of dislocation structures and grain fragmentation at the bonding interface when

sufficient and necessary boundary conditions pertaining to the Ultrasonic Consolidation (UC)

process are prescribed.

The hardening is incorporated using statistically stored and geometrically necessary

dislocation densities (SSDs and GNDs) which are dislocation analogs of isotropic and kinematic

hardening respectively. Since, the macroscopic boundary conditions during UC involves cyclic

sinusoidal simple shear loading along with constant normal pressure, the cross slip mechanism

has been included in the evolution equation for SSDs. The inclusion of cross slip promotes slip

irreversibility, dislocation storage and, hence, cyclic hardening during the UC. The GND

considers strain-gradient and thus renders the model size-dependent. The model is calibrated

using experimental data from published refereed literature for simple shear deformation of single

crystalline pure aluminum alloy and uniaxial tension of polycrystalline Aluminum 3003-H18

alloy. The model also considers the tension-compression asymmetry in case the model is applied

for deformation processes in hexagonal close packed pure Titanium and its alloy counterparts

which will be investigated further in our proposed research program. One of the significant

macroscopic contributions from this model development is to successfully accommodate the

elasto-plastic contact problem involved in UC.

The model also incorporates various local and global effects such as friction, thermal

softening, acoustic softening, surface texture of the sonotrode and initial mating surfaces and

presence of oxide-scale at the mating surfaces which further contribute significantly specifically

to the grain substructure evolution at the interface and to the anisotropic bulk deformation away

from the interface during UC in general. The model results have been predicted for Al-3003 H-

18 alloy undergoing UC. A good agreement between the experimental and simulated results has

been observed for the evolution of linear weld density and anisotropic global strengths

macroscopically. Similarly, microscopic observations such as embrittlement due to grain

substructure evolution and broken oxide layer at the UC interface has been also demonstrated by

the simulation.

Introduction

As a direct result of ongoing research efforts in ultrasonic consolidation (UC) worldwide, it has

become apparent that a new approach to modeling of UC bonding is needed. A model which

provides a better understanding of the effects of process parameter changes on grain refinement,

375

bjfTypewritten TextREVIEWED, August 17 2011

plastic deformation and bonding during UC will better enable researchers to predict which

materials will bond, how the mechanical properties of UC-produced parts can be improved, and

how to better design the next generation of UC equipment.

The continuum properties of parts made using UC are strongly dependent upon the

micromechanics of the bonded interface [1]. Interfacial-scale microstructures can be studied

fundamentally using electron microscopy and can be used to correlate atomic and mesoscopic

mechanisms of deformation to their continuum counterparts. A dislocation density-based crystal

plasticity finite element model (DDCP-FEM) can capture the statistical distribution of

dislocations, partials and various deformation mechanisms at the bonding interface as inputs to

predict macroscopic deformation and mechanical property profiles as a function of energy input

characteristics. These input characteristics are a function of the process parameters used in a UC

machine, namely vibration amplitude, normal force, ultrasonic frequency, welding speed,

sonotrode geometry and temperature.

Problem Formulation

It has been shown that material sheets subjected to UC undergo inhomogeneous plastic

deformation through their thickness [1]. Classical continuum plasticity theories do not fully

explain this phenomenon [2]. Therefore, a study of strain localization and grain refinement at the

material interfaces during UC bonding is required. The following steps lead to the calculation of

these localized strains and their effects.

1 Large Deformation Quasi-static formulation

The deformation map in space and time is described by the total deformation gradient

tensor F (Figure 1). Applying the Kroner-Lee assumption, F is decomposed into elastic Fe and

plastic gradient Fp tensors using multiplicative operator theory

(Eqn 1)

The plastic deformation gradient Fp includes constant volume plastic deformation

without disturbance of the crystal lattice. Elastic distortion and rigid rotation of the lattice are

described by a unique intermediate configuration free of local stresses.

2 The non-local dislocation density motivated material model

The flow response for dislocation density motivated crystal plasticity modeling in a given

slip system '' is given by (Ma 2006):

{

*

(

| |

)+ (

)

| |

| |

(Eqn 2)

376

where the pre-exponential variable is the upper limit of the shear rate for the case where the

Boltzmann factor is equal to 1, which can be found using:

(Eqn 3)

Figure1 Multiplicative decomposition of the total deformation gradient, F=FeFp. The rotation

and stretching of the lattice are taken into account through the elastic deformation gradient Fe

[3].

and the passing stress, , caused by parallel dislocations can be found using:

(Eqn 4)

and the cutting stress, , at 0K caused by forest dislocations can be found using:

(Eqn5)

where Qslip is the effective activation energy for dislocation slip.

The incompatibility in plastic deformation gradient and non-local geometrical non-

linearity is introduced using which computes the geometrically necessary dislocations

required to maintain continuity throughout the material. The evolution law for is:

(

) (Eqn6)

377

Material hardening at an integration point is both a function of and

(statistically stored dislocation density). The evolution laws for are generally linear in shear

rate (Eqn7).

(

)| |

( ) ( )

(Eqn7)

The various constants used in this modeling can be attributed to physical phenomena as

shown in Table 1.

Material Parameter Physical Meaning Prescribed Value

Qslip Energy barrier for slip 3.0x10-19

J

Qbulk Energy barrier for climb (activated

at higher temperatures)

2.4x10-19

J

c1 constant for passing stress (due to in-

plane dislocations) (Equation 3)

0.1

c2 constant for jump width (Equation 4) 2.0

c3 constant for obstacle width

(Equation 4)

1.0

c4 constant for lock forming rate

(Equation 7)

1.5x107m

-1

c5 constant for athermal annihilation

rate (Equation 7)

10.0

c6 constant for dipole forming rate

(Equation 7)

1.0x10-30

m-1

c7 constant for thermal annihilation rate

(Equation 7)

1x107m

5c

8

c8 constant for non-linear climb of edge

dislocation (Equation 7)

0.3

c9 constant for energy scaling at the

interface

10-3

Table1 Physical Interpretation for various constants used in the Constitutive model

378

3 Global and Local Solution Strategies

The global and local solution strategy developed for solving the crystal plasticity

constitutive model in section 2.2 is shown in Table 2.

Table2 Solution strategy for solving the crystal plasticity constitutive model with Nonlinear

FEM.

First, the applied loading is applied incrementally as load steps. At the beginning of each

load step (k+1), various nodal and integration point variables such as displacement ( ), plastic deformation gradient ( ), SSD and GND are initialized to their converged counterparts obtained in the previous load step. After initialization, an iterative procedure is used to solve for the local

integration point variables. In every iteration (i), a local integration is performed via the B-Bar

scheme to compute the stress, plastic deformation gradient and the hardness due to immobilized

dislocation content (SSD). The stress is then resolved on a slip system to obtain the resolved

shear stress (RSS, ) followed by plastic shear strain rate which further leads to the calculation of

*View more*